General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.56 - 7.7 g/cm³ Show Material materials with Density of 7.56 - 7.7 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | 20.0 °C | 218 - 220 GPa Show Material materials with Elastic modulus of 218 - 220 GPa | |

100.0 °C | 213 - 215 GPa Show Material materials with Elastic modulus of 213 - 215 GPa | ||

200.0 °C | 206 - 210 GPa Show Material materials with Elastic modulus of 206 - 210 GPa | ||

300.0 °C | 198 - 205 GPa Show Material materials with Elastic modulus of 198 - 205 GPa | ||

400.0 °C | 190 - 195 GPa Show Material materials with Elastic modulus of 190 - 195 GPa | ||

500.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | ||

600.0 °C | 167 GPa Show Material materials with Elastic modulus of 167 GPa | ||

700.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | ||

Elongation | 20.0 °C | 23 % Show Material materials with Elongation of 23 % | |

Elongation A80 | 20.0 °C | 23 % Show Material materials with Elongation A80 of 23 % | |

Elongation A80, transverse | 20.0 °C | 23 % Show Material materials with Elongation A80, transverse of 23 % | |

Elongation, transverse | 20.0 °C | 23 % Show Material materials with Elongation, transverse of 23 % | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Ferritic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Ferritic Stainless Steel |

Tensile strength | 20.0 °C | 420 - 600 MPa Show Material materials with Tensile strength of 420 - 600 MPa | |

Tensile strength, transverse | 20.0 °C | 420 - 600 MPa Show Material materials with Tensile strength, transverse of 420 - 600 MPa | |

Yield strength Rp0.2 | 20.0 °C | 230 MPa Show Material materials with Yield strength Rp0.2 of 230 MPa | |

100.0 °C | 195 MPa Show Material materials with Yield strength Rp0.2 of 195 MPa | ||

150.0 °C | 190 MPa Show Material materials with Yield strength Rp0.2 of 190 MPa | ||

200.0 °C | 185 MPa Show Material materials with Yield strength Rp0.2 of 185 MPa | ||

250.0 °C | 175 MPa Show Material materials with Yield strength Rp0.2 of 175 MPa | ||

300.0 °C | 165 MPa Show Material materials with Yield strength Rp0.2 of 165 MPa | ||

350.0 °C | 155 MPa Show Material materials with Yield strength Rp0.2 of 155 MPa | ||

Unlock all property charts | |||

Yield strength Rp0.2, transverse | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp0.2, transverse of 240 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 20.0 °C | 9.9E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.9E-6 1/K | |

100.0 °C | 1E-5 - 1.03E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 - 1.03E-5 1/K | ||

200.0 °C | 1E-5 - 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 - 1.08E-5 1/K | ||

300.0 °C | 1.05E-5 - 1.12E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 - 1.12E-5 1/K | ||

400.0 °C | 1.05E-5 - 1.16E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 - 1.16E-5 1/K | ||

500.0 °C | 1.1E-5 - 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.1E-5 - 1.19E-5 1/K | ||

600.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

700.0 °C | 1.24E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.24E-5 1/K | ||

800.0 °C | 1.29E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1425 - 1530 °C Show Material materials with Melting point of 1425 - 1530 °C | Typical for Ferritic Stainless Steel | |

Specific heat capacity | 20.0 °C | 450 - 460 J/(kg·K) Show Material materials with Specific heat capacity of 450 - 460 J/(kg·K) | |

100.0 °C | 482 J/(kg·K) Show Material materials with Specific heat capacity of 482 J/(kg·K) | ||

200.0 °C | 506 J/(kg·K) Show Material materials with Specific heat capacity of 506 J/(kg·K) | ||

300.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | ||

400.0 °C | 547 J/(kg·K) Show Material materials with Specific heat capacity of 547 J/(kg·K) | ||

500.0 °C | 576 J/(kg·K) Show Material materials with Specific heat capacity of 576 J/(kg·K) | ||

600.0 °C | 616 J/(kg·K) Show Material materials with Specific heat capacity of 616 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 16 - 25 W/(m·K) Show Material materials with Thermal conductivity of 16 - 25 W/(m·K) | |

100.0 °C | 17.2 W/(m·K) Show Material materials with Thermal conductivity of 17.2 W/(m·K) | ||

200.0 °C | 18.6 W/(m·K) Show Material materials with Thermal conductivity of 18.6 W/(m·K) | ||

300.0 °C | 20 W/(m·K) Show Material materials with Thermal conductivity of 20 W/(m·K) | ||

400.0 °C | 21.2 W/(m·K) Show Material materials with Thermal conductivity of 21.2 W/(m·K) | ||

500.0 °C | 22.3 W/(m·K) Show Material materials with Thermal conductivity of 22.3 W/(m·K) | ||

600.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

700.0 °C | 24.1 W/(m·K) Show Material materials with Thermal conductivity of 24.1 W/(m·K) | ||

800.0 °C | 25.5 W/(m·K) Show Material materials with Thermal conductivity of 25.5 W/(m·K) | ||

900.0 °C | 26.9 W/(m·K) Show Material materials with Thermal conductivity of 26.9 W/(m·K) | ||

1000.0 °C | 28.3 W/(m·K) Show Material materials with Thermal conductivity of 28.3 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | |

100.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

200.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.4 mm²/s Show Material materials with Thermal diffusivity of 4.4 mm²/s | ||

500.0 °C | 4.1 mm²/s Show Material materials with Thermal diffusivity of 4.1 mm²/s | ||

600.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 6E-7 - 9.06E-7 Ω·m Show Material materials with Electrical resistivity of 6E-7 - 9.06E-7 Ω·m |

100.0 °C | 9.42E-7 Ω·m Show Material materials with Electrical resistivity of 9.42E-7 Ω·m | |

200.0 °C | 9.87E-7 Ω·m Show Material materials with Electrical resistivity of 9.87E-7 Ω·m | |

300.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m | |

400.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

500.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

600.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

700.0 °C | 1.22E-6 Ω·m Show Material materials with Electrical resistivity of 1.22E-6 Ω·m | |

800.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

900.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

1000.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.05 % Show Material materials with Carbon of 0.05 % |

Chromium | 16 - 18 % Show Material materials with Chromium of 16 - 18 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Titanium | 0.8 % Show Material materials with Titanium of 0.8 % |